Chapter 5: Diffusion. 5.1 SteadyState Diffusion


 Ashlee Carpenter
 1 years ago
 Views:
Transcription
1 : Diffusion Diffusion: the movement of particles in a solid from an area of high concentration to an area of low concentration, resulting in the uniform distribution of the substance Diffusion is process which is NOT due to the action of a force, but a result of the random movements of atoms (statistical problem) 1. Diffusivity and Fick s laws. Atomistic mechanisms of diffusion 3. Temperature dependence and Arrenius plot 4. Industrial applications  carburized steel,  dopants in silicon 5.1 SteadyState Diffusion Consider diffusion of solute atoms (b) in solid state solution (AB) in direction between two parallel atomic planes (separated by ) if there is no changes with time in C B at these planes such diffusion condition is called steadystate diffusion For a steadystate diffusion, flu (flow), J, of atoms is: dc J = D d J flu of atoms, atoms/(m s): the number of particles which pass through a unit area in a unit of time; D diffusivity or diffusion coefficient, m /s dc/d concentration gradient, atoms/m 4 Recall: Solvent the majority atom type (or host atoms): Solute the element with lower concentration Substitutional a solid solution in which the solute atoms are replaced by solute Interstitial solute atoms are located in gaps between host atoms 1
2 Fick s first law of diffusion dc J = D d atoms m J = D m s s  sign: flu direction is from the higher to the lower concentration; i.e. it is the opposite to the concentration gradient For steadystate diffusion condition (no change in the system with time), the net flow of atoms is equal to the diffusivity D times the diffusion gradient dc/d dc atoms 1 3 d m m Diffusivity D depends on: 1. Diffusion mechanism. Temperature of diffusion 3. Type of crystal structure (bcc > fcc) 4. Crystal imperfections 5. Concentration of diffusing species NonSteadyState Diffusion In practice the concentration of solute atoms at any point in the material changes with time nonsteadystate diffusion For nonsteadystate condition, diffusion coefficient, D  NOT dependent on time: Second Fick s law of diffusion: If D D(), in 1D case: dc dt = dc dt d d dc D d C = D Change in concentration in semiinfinite rods of Cu and Ni caused by diffusion, From G. Gottstein Physical Foundations of Material Science The rate of compositional change is equal to the diffusivity times the rate of the change of the concentration gradient In 3D case: dc dt C C C D + + y z =
3 NonSteadyState Diffusion (continued) With specific initial or boundary conditions this partial differential equations can be solved to give the concentration as function of spatial position and time c(, y, z, t) Let us consider two rods with different concentrations c 1 and c which are joined at =0 and both are so long that mathematically they can be considered as infinitely long The concentration profile at t = 0 is discontinuous at = 0: < 0, c = c 1 ; < 0, c = c dc We can obtain solution of: C = D dt c c(, t) c = where erf ( z) = z = Dt 1 c π 1 π z 0 Dt e e ξ ξ c dξ = c erf Dt dξ, is known as the error function Gas diffusion into a solid Let us consider the case of a gas A diffusing into a solid B Gas A Solid B Cs C C C S o = erf Dt = 0 C S surf. C of element in gas diffusing into the surface C o initial uniform concentration of element in solid  distance from surface D diffusivity of diffusing solute element t time erf mathematical function called error function 3
4 Error function Curve of the error function erf (z) for z = Dt Q: Consider the gas carburizing of a gear of 1018 steel (C 0.18 wt %) at 97 C. Calculate the time necessary to increase the C content to 0.35 wt % at 0.40 mm below the surface of the gear. Assume the C content at the surface to be 1.15 wt % and that the nominal C content of the steel gear before carburizing is 0.18 wt %. D (C in γ iron) at 97 C = m /s 4
5 5. Atomistics of Solid State Diffusion Diffusion mechanisms: 1. Vacancy (substitutional) diffusion migration of atom in a lattice assisted by the presence of vacancies E.: self diffusion of Cu atoms in Cu crystal. Interstitial diffusion movement of atoms from one interstitial site to another neighboring interstitial site without permanent displacement any of the atoms in the matri crystal lattice E.: C diffusion in BCC iron Vacancies The simplest point defect is the vacancy (V) an atom site from which an atom is missing Vacancies are always present; their number N V depends on temperature (T) N V = N e EV kt N V  # of vacancies N  number of lattice sites E V energy required to form a vacancy k Boltzmann constant k = J K 1 ; or ev K 1 T absolute temperature vacancy 5
6 Vacancy (Substitutional) Diffusion Mechanism Substitutional (in homogeneous system  selfdiffusion, in heterogeneous system solid state solutions) Vacancies are always present at any T As T increases # of vacancies increases diffusion rate increases Move atom A (from (1) to ()) = move vacancy from () to (1)..? higher T melt stronger bonding between atoms high activation energy to move V Kirkendall effect Marker at the diffusion interface move slightly in the opposite direction to the most rapidly moving species vacancies can move! 6
7 Possible mechanisms of selfdiffusion and their activation energy 1. Neighboring atoms echange sites. Ring mechanism 3. Vacancy mechanism 4. Direct interstitial mechanism 5. Indirect interstitial mechanism Migration Formation Total ev 1 ev  1 ev 8 ev ev ev 3.4 ev 4 ev 6 0. ev 3.4 ev 3.6 ev Anisotropy Effects From G.Gottstein Physical Foundations of Material Science 7
8 Carbon diffusion in Fe Jump frequency Γ [s 1 ] of an atom is given by: Γ = ν kt e G m Usually ν [s 1 ] vibrational frequency of the atom There is a fundamental relationship between the jump frequency Γ and the diffusion coefficient D which is independent of mechanism and crystal structure: λ λ D = Γ = 6 6τ λ the jump distance of the diffusing atom τ =1/Γ the time interval between two jumps J = J MN  J NM A 1 J = C M Γ C 4 3 D = Γa 4 A N 1 Γ 4 3 Carbon diffusion in Fe Can be derived from an atomistic considerations of the diffusion processes C atoms are located on the octahedral interstitial sites (black circles) J = J MN  J NM Only ¼ of possible jumps of C atoms lead to flu in + Only /3 of all C atoms can jump in direction λ λ D = Γ = 6 6τ D = Γa 4 8
9 5.3 Effects of T on diffusion in solids Diffusion rate in a system will increase with temperature: D = D e o EA RT D diffusivity, m /s D 0 proportionality constant, m /s, independent of T E A activation energy for diffusing species, J/mol R molar gas constant R = J mol1 K1; or 1.987cal mol1k1 T absolute temperature Activation energy A + B C + D A (initial state) A* (final state) only a fraction of the molecules or atoms in a system will have sufficient energy to reach E* A thermally active process is one which requires a definite amount of thermal energy to overcome an activation energy barrier and enter the reactive state 9
10 Bolzmann s equation On the basis of statistical analysis, Bolzmann s results showed that the probability of finding a molecule or atom at an energy level E * > the average energy E of all the molecules or atoms in a system at a particular temperature T, K, was: Probability e * E E kt where k B = J/(atom K)  Boltzmann s constant The fraction of atoms or molecules in a system having energies > E* at a given T (where E* is much greater than the average energy of any atom or molecule: n N total = C e * E kt Arrhenius Rate Equation The rate of many chemical reaction as a function of temperature as follows: Rate _ of _ reaction = C e E A RT C rate constant, independent of T E A activation energy R molar gas constant R = J mol 1 K 1 ; or 1.987cal mol 1 K 1 T absolute temperature 10
11 If we rewrite in natural log plot: EA ln rate = ln C RT ln rate = a ln C = b y = b + m 1 = T Typical Arrhenius Plot or in logarithmic log plot: log rate = log10 C 10 EA.303RT Q.: The diffusivity of Ag atoms in solid silver metal is 1.0X10 17 m /s at 500 o C and m /s at 1000 o C. Calculate the activation energy (J/mole) for the diffusion of Ag in Ag in the T range 500 to 1000 o C. 11
12 5.4 Industrial applications Steel Hardening by Gas Carburizing In the gas carburizing process for steel parts, the parts are placed in a furnace in contact with a gas rich in COCH 4 miture at ~97ºC. Fe + CH 4 FeC ( = % C), T = 97 o C The C from the gas diffuses into the surface of the steel part and increases the C content of the outer surface region of the part. The higher C concentration at the surface makes the steel harder in this region A steel part can thus be produced with a hard outer layer and a tough low C steel inner core (important, for eample, for many types of gears) Dopants activation Dopants can be incorporated into Si wafer to change their electrical conducting characteristics mask B, P + Ion implantation Annealing 1
13 Q: If boron, B, is diffused into a thick slice of Si with no previous B in it at a temperature of 1100 C for 5 h, what is the depth below the surface at which the concentration is atoms/cm 3 if the surface concentration is atoms/cm3? D = cm /s for B diffusing in Si at 1100 C. Summary Diffusion: the movement of particles in a solid from an area of high concentration to an area of low concentration, resulting in the uniform distribution of the substance Fick s first diffusion law: for steadystate diffusion condition (no change in the system with time), the net flow of atoms is equal to the diffusivity D times the diffusion gradient dc/d J = D Fick s second diffusion law: The rate of compositional change is equal to the diffusivity times the rate of the change of the concentration gradient Diffusion rate in a system will increase with temperature: D = D e o dc d dc C = D dt EA RT 13
Chapter Outline. Diffusion  how do atoms move through solids?
Chapter Outline iffusion  how do atoms move through solids? iffusion mechanisms Vacancy diffusion Interstitial diffusion Impurities The mathematics of diffusion Steadystate diffusion (Fick s first law)
More informationTHE WAY TO SOMEWHERE. Subtopics. Diffusion Diffusion processes in industry
THE WAY TO SOMEWHERE Subtopics 1 Diffusion Diffusion processes in industry RATE PROCESSES IN SOLIDS At any temperature different from absolute zero all atoms, irrespective of their state of aggregation
More informationIntroduction To Materials Science FOR ENGINEERS, Ch. 5. Diffusion. MSE 201 Callister Chapter 5
Diffusion MSE 21 Callister Chapter 5 1 Goals: Diffusion  how do atoms move through solids? Fundamental concepts and language Diffusion mechanisms Vacancy diffusion Interstitial diffusion Impurities Diffusion
More informationIn order to solve this problem it is first necessary to use Equation 5.5: x 2 Dt. = 1 erf. = 1.30, and x = 2 mm = 2 103 m. Thus,
5.3 (a) Compare interstitial and vacancy atomic mechanisms for diffusion. (b) Cite two reasons why interstitial diffusion is normally more rapid than vacancy diffusion. Solution (a) With vacancy diffusion,
More informationLecture 3: Introduction to Diffusion
Materials Science & Metallurgy Master of Philosophy, Materials Modelling, Course MP6, Kinetics and Microstructure Modelling, H. K. D. H. Bhadeshia Lecture 3: Introduction to Diffusion Mass transport in
More informationMAE 20 Winter 2011 Assignment 3 solutions
MAE 20 Winter 2011 Assignment 3 solutions 4.3 Calculate the activation energy for vacancy formation in aluminum, given that the equilibrium number of vacancies at 500 C (773 K) is 7.57 10 23 m 3. The
More informationDIFFUSION IN SOLIDS. Materials often heat treated to improve properties. Atomic diffusion occurs during heat treatment
DIFFUSION IN SOLIDS WHY STUDY DIFFUSION? Materials often heat treated to improve properties Atomic diffusion occurs during heat treatment Depending on situation higher or lower diffusion rates desired
More informationMaterials Science and Engineering Department MSE , Sample Test #1, Spring 2010
Materials Science and Engineering Department MSE 200001, Sample Test #1, Spring 2010 ID number First letter of your last name: Name: No notes, books, or information stored in calculator memories may be
More information14:635:407:02 Homework III Solutions
14:635:407:0 Homework III Solutions 4.1 Calculate the fraction of atom sites that are vacant for lead at its melting temperature of 37 C (600 K). Assume an energy for vacancy formation of 0.55 ev/atom.
More informationCh. 4: Imperfections in Solids Part 1. Dr. Feras Fraige
Ch. 4: Imperfections in Solids Part 1 Dr. Feras Fraige Outline Defects in Solids 0D, Point defects vacancies Interstitials impurities, weight and atomic composition 1D, Dislocations edge screw 2D, Grain
More informationDefects Introduction. Bonding + Structure + Defects. Properties
Defects Introduction Bonding + Structure + Defects Properties The processing determines the defects Composition Bonding type Structure of Crystalline Processing factors Defects Microstructure Types of
More informationCHAPTER 4 IMPERFECTIONS IN SOLIDS PROBLEM SOLUTIONS
41 CHAPTER 4 IMPERFECTIONS IN SOLIDS PROBLEM SOLUTIONS Vacancies and SelfInterstitials 4.1 In order to compute the fraction of atom sites that are vacant in copper at 1357 K, we must employ Equation
More informationImperfections in atomic arrangements
MME131: Lecture 8 Imperfections in atomic arrangements Part 1: 0D Defects A. K. M. B. Rashid Professor, Department of MME BUET, Dhaka Today s Topics Occurrence and importance of crystal defects Classification
More informationSurface Treatments. Corrosion Protective coatings for harsh environments (catalytic converters, electrochemical cells )
Surface Treatments Applications Biomedical (biocompatible coatings on implants, drug coatings for sustained release ) Mechanical Tribological friction and wear (tool steels, implants ) Fatigue minimize
More informationCHAPTER 6: DIFFUSION IN SOLIDS. Interdiffusion. Simple Diffusion. Diffusion Steady and NonSteady State ISSUES TO ADDRESS...
CHAPTER 6: DIFFUSION IN SOLIDS Diffusion Steady and NonSteady State ISSUES TO ADDRESS... Gear from casehardened steel (C diffusion) Diffusion  Mass transport by atomic motion How does diffusion occur?
More informationSolution: ΔG = a 3 ΔG v. + 6a 2 γ. Differentiation of this expression with respect to a is as. d ΔG da = d(a3 ΔG v. + d(6a2 γ) = 3a 2 ΔG v.
14:440:407 ch10 Question 10.2: (a) Rewrite the expression for the total free energy change for nucleation (Equation 10.1) for the case of a cubic nucleus of edge length a (instead of a sphere of radius
More informationThe University of Western Ontario Department of Physics and Astronomy P2800 Fall 2008
P2800 Fall 2008 Questions (Total  20 points): 1. Of the noble gases Ne, Ar, Kr and Xe, which should be the most chemically reactive and why? (0.5 point) Xenon should be most reactive since its outermost
More information in a typical metal each atom contributes one electron to the delocalized electron gas describing the conduction electrons
Free Electrons in a Metal  in a typical metal each atom contributes one electron to the delocalized electron gas describing the conduction electrons  if these electrons would behave like an ideal gas
More informationThe atomic packing factor is defined as the ratio of sphere volume to the total unit cell volume, or APF = V S V C. = 2(sphere volume) = 2 = V C = 4R
3.5 Show that the atomic packing factor for BCC is 0.68. The atomic packing factor is defined as the ratio of sphere volume to the total unit cell volume, or APF = V S V C Since there are two spheres associated
More informationMechanical Properties of Metals Mechanical Properties refers to the behavior of material when external forces are applied
Mechanical Properties of Metals Mechanical Properties refers to the behavior of material when external forces are applied Stress and strain fracture or engineering point of view: allows to predict the
More informationChapter 3: Kinetics of Electrode Reactions
Goal: To understand the observed behavior of electrode kinetics with respect to potential and concentration. = i/nfa (mol/scm 2 ) Rate = f(e) Dynamic Equilibrium A k f k b B s 1 f = k f C A (M/s) b =
More informationVysoká škola báňská Technická univerzita Ostrava. Physical Metallurgy. Didactic Text. Jaroslav Sojka
Vysoká škola báňská Technická univerzita Ostrava Physical Metallurgy Didactic Text Jaroslav Sojka Ostrava 2013 Physical Metallurgy Review: Prof. Ing. Ludmila Hypecká, DrSc. Description: Physical Metallurgy
More informationMechanisms of Diffusion in Materials 3.205 L4 11/7/06
Mechanisms of Diffusion in Materials 1 A final point on interdiffusion The composition profiles resulting from interdiffusion are generally constrained by phase equilibria. Consider the an Ir Re diffusion
More informationChapter Outline: Phase Transformations in Metals
Chapter Outline: Phase Transformations in Metals Heat Treatment (time and temperature) Microstructure Mechanical Properties Kinetics of phase transformations Multiphase Transformations Phase transformations
More informationChapter Outline. Defects Introduction (I)
Crystals are like people, it is the defects in them which tend to make them interesting!  Colin Humphreys. Defects in Solids Chapter Outline 0D, Point defects vacancies interstitials impurities, weight
More informationChapter Outline Dislocations and Strengthening Mechanisms
Chapter Outline Dislocations and Strengthening Mechanisms What is happening in material during plastic deformation? Dislocations and Plastic Deformation Motion of dislocations in response to stress Slip
More informationMet2023: Concepts of Materials Science I Sample Questions & Answers,(2009) ( Met, PR, FC, MP, CNC, McE )
1 Met223: Concepts of Materials Science I Sample Questions & Answers,(29) ( Met, PR, FC, MP, CNC, McE ) Q1.Define the following. (i) Point Defects (ii) Burgers Vector (iii) Slip and Slip system (iv)
More informationPhase Transformations in Metals and Alloys
Phase Transformations in Metals and Alloys THIRD EDITION DAVID A. PORTER, KENNETH E. EASTERLING, and MOHAMED Y. SHERIF ( г йс) CRC Press ^ ^ ) Taylor & Francis Group Boca Raton London New York CRC Press
More informationIronCarbon Phase Diagram (a review) see Callister Chapter 9
IronCarbon Phase Diagram (a review) see Callister Chapter 9 University of Tennessee, Dept. of Materials Science and Engineering 1 The Iron Iron Carbide (Fe Fe 3 C) Phase Diagram In their simplest form,
More informationChapter Outline Dislocations and Strengthening Mechanisms
Chapter Outline Dislocations and Strengthening Mechanisms What is happening in material during plastic deformation? Dislocations and Plastic Deformation Motion of dislocations in response to stress Slip
More informationCHAPTER 7 DISLOCATIONS AND STRENGTHENING MECHANISMS PROBLEM SOLUTIONS
71 CHAPTER 7 DISLOCATIONS AND STRENGTHENING MECHANISMS PROBLEM SOLUTIONS Basic Concepts of Dislocations Characteristics of Dislocations 7.1 The dislocation density is just the total dislocation length
More informationv kt = N A ρ Au exp (
42 4.2 Determination of the number of vacancies per cubic meter in gold at 900 C (1173 K) requires the utilization of Equations 4.1 and 4.2 as follows: N v N exp Q v N A ρ Au kt A Au exp Q v kt (6.023
More informationProcessing of Semiconducting Materials Prof. Pallab Banerji Department of Metallurgy and Material Science Indian Institute of Technology, Kharagpur
Processing of Semiconducting Materials Prof. Pallab Banerji Department of Metallurgy and Material Science Indian Institute of Technology, Kharagpur Lecture  8 Diffusion and Ion Implantation II (Refer
More informationChapter 8. Phase Diagrams
Phase Diagrams A phase in a material is a region that differ in its microstructure and or composition from another region Al Al 2 CuMg H 2 O(solid, ice) in H 2 O (liquid) 2 phases homogeneous in crystal
More informationELECD Principles of materials science Thermodynamics and diffusion. ELECD Principles of materials science
Thu 3.3 Mon 7.3 ELECD8710  Principles of materials science Thermodynamics and diffusion Thu 10.3 Exercise 5 Mon 14.3 Thu 17.3 Exercise 6 Mon 21.3 Thermodynamics  Principles (T,xi) equilibrium diagrams
More informationModule  01 Lecture  23 The Diffusion Equation
Electronic Materials Devices and Fabrication Layering: Thermal Oxidation Dr. S. Parasuraman Department of Metallurgical and Materials Engineering Indian Institute of Technology, Madras Module  01 Lecture
More informationKinetic Molecular Theory of Matter
Kinetic Molecular Theor of Matter Heat capacit of gases and metals Pressure of gas Average speed of electrons in semiconductors Electron noise in resistors Positive metal ion cores Free valence electrons
More informationCh 3. Rate Laws and Stoichiometry
Ch 3. Rate Laws and Stoichiometry How do we obtain r A = f(x)? We do this in two steps 1. Rate Law Find the rate as a function of concentration, r A = k fn (C A, C B ). Stoichiometry Find the concentration
More informationQuestion 6.5: A steel bar 100 mm (4.0 in.) long and having a square cross section 20 mm
14:440:407 Ch6 Question 6.3: A specimen of aluminum having a rectangular cross section 10 mm 12.7 mm (0.4 in. 0.5 in.) is pulled in tension with 35,500 N (8000 lb f ) force, producing only elastic deformation.
More informationReaction Mechanism (continued) CHEMICAL KINETICS. Pt 2. Reaction Mechanisms. Often Used Terms. Reaction Mechanisms. The reaction
Reaction Mechanism (continued) CHEMICAL KINETICS Pt The reaction C H O + 5O 6CO + 4H O 3 4 3 has many steps in the reaction mechanism. Objectives! Be able to describe the collision and transitionstate
More informationSolidliquid Interface Energy of Metals at Melting Point and Undercooled State
Materials ransactions, Vol. 43, No. 4 (2002) pp. 721 to 726 c 2002 he Japan Institute of Metals Solidliquid Interface Energy of Metals at Melting Point and Undercooled State Zengyun Jian 1, Kazuhiko Kuribayashi
More informationRef. Ch. 11 in Superalloys II Ch. 8 in Khanna Ch. 14 in Tien & Caulfield
MTE 585 Oxidation of Materials Part 1 Ref. Ch. 11 in Superalloys II Ch. 8 in Khanna Ch. 14 in Tien & Caulfield Introduction To illustrate the case of high temperature oxidation, we will use Nibase superalloys.
More informationFigure 10.1. Process flow from starting material to polished wafer.
Figure 10.1. Process flow from starting material to polished wafer. 1/11/003 Ettore Vittone Fisica dei Semiconduttori  Lectio XI 1 Starting material: silicon dioxide (SiO ): pure form of sand (quartzite)
More informationChapter 14 Chemical Kinetics
Chapter 14 Chemical Kinetics Chemical kinetics: the area of chemistry dealing with the speeds or rates at which reactions occur. Rates are affected by several factors: The concentrations of the reactants:
More informationChemical Kinetics. Reaction Rate: The change in the concentration of a reactant or a product with time (M/s). Reactant Products A B
Reaction Rates: Chemical Kinetics Reaction Rate: The change in the concentration of a reactant or a product with time (M/s). Reactant Products A B change in number of moles of B Average rate = change in
More informationPhysical Vapor Deposition (PVD): SPUTTER DEPOSITION
We saw CVD PECVD Physical Vapor Deposition (PVD): SPUTTER DEPOSITION Gas phase reactants: P g 1 mtorr to 1 atm. Good step coverage, T > > RT Plasma enhanced surface diffusion without need for elevated
More informationPhysics 610/Chemistry 678 Semiconductor Processing and Characterization Quiz I July 18, 2014
Physics 610/Chemistry 678 Semiconductor Processing and Characterization Quiz I July 18, 2014 Part I: Shortanswer questions on basic principles. (5 points each) 1. Briefly describe the CZ method and the
More informationChapter 13 Properties of Solutions. Classification of Matter
Chapter 13 Properties of Solutions Learning goals and key skills: Describe how enthalpy and entropy changes affect solution formation Describe the relationship between intermolecular forces and solubility,
More informationCHAPTER 4 IMPERFECTIONS IN SOLIDS PROBLEM SOLUTIONS. C Zn A Cu C Zn A Cu C Cu A Zn. (30)(63.55 g /mol) (30)(63.55 g /mol) (70)(65.
HAPTER 4 IMPERFETIONS IN SOLIDS PROBLEM SOLUTIONS wt% u? 4.7 What is the composition, in atom percent, of an alloy that consists of 30 wt% Zn and 70 4.6 as In order to compute composition, in atom percent,
More informationFatigue :Failure under fluctuating / cyclic stress
Fatigue :Failure under fluctuating / cyclic stress Under fluctuating / cyclic stresses, failure can occur at loads considerably lower than tensile or yield strengths of material under a static load: Fatigue
More informationLecture 12. Physical Vapor Deposition: Evaporation and Sputtering Reading: Chapter 12. ECE 6450  Dr. Alan Doolittle
Lecture 12 Physical Vapor Deposition: Evaporation and Sputtering Reading: Chapter 12 Evaporation and Sputtering (Metalization) Evaporation For all devices, there is a need to go from semiconductor to metal.
More informationCHEMICAL KINETICS (RATES OF REACTION)
1 CHEMICAL KINETICS (RATES OF REACTION) Introduction Chemical kinetics is concerned with the dynamics of chemical reactions such as the way reactions take place and the rate (speed) of the process. Collision
More informationUniversity of Cambridge, Materials Science & Metallurgy. Dilatometry
University of Cambridge, Materials Science & Metallurgy H. K. D. H. Bhadeshia Dilatometry The dilatometric method utilises either transformation strains or thermal strains; the basic data generated are
More informationCrystal Structure and Growth
Crystal Structure and Growth Source: USNA EE 452 Course on IC Technology EE452 131 Atomic Order of a Crystal Structure EE452 132 Amorphous Atomic Structure EE452 133 Unit Cell in 3D Structure Unit
More informationphys4.17 Page 1  under normal conditions (pressure, temperature) graphite is the stable phase of crystalline carbon
Covalent Crystals  covalent bonding by shared electrons in common orbitals (as in molecules)  covalent bonds lead to the strongest bound crystals, e.g. diamond in the tetrahedral structure determined
More informationBasic laws and electrical properties of metals (I) Electrical properties. Basic laws and electrical properties of metals (II)
Electrical properties Electrical conduction How many moveable electrons are there in a material (carrier density)? How easily do they move (mobility)? Semiconductivity Electrons and holes Intrinsic and
More informationFree Electron Fermi Gas (Kittel Ch. 6)
Free Electron Fermi Gas (Kittel Ch. 6) Role of Electrons in Solids Electrons are responsible for binding of crystals  they are the glue that hold the nuclei together Types of binding (see next slide)
More informationChemistry 4th Edition McMurry/Fay
13 Ch a pt e r Chemical Equilibrium Chemistry 4th Edition McMurry/Fay Dr. Paul Charlesworth Michigan Technological University The Equilibrium State 01 Chemical Equilibrium: A state achieved when the rates
More informationPhase Transformations
Vysoká škola báňská Technická univerzita Ostrava Phase Transformations Didactic Text Vlastimil Vodárek Ostrava 2013 Review: Prof. Dr. Ing. Jaroslav Sojka Description: Phase Transformations Author: Vlastimil
More informationFACTORS AFFECTING REACTION RATES
QUESTIONSHEET 1 a) Rate at which the molar concentration of a reactant decreases with time FACTORS AFFECTING REACTION RATES Or r =  dc dt where dc is a concentration change occurring in a time interval
More informationLecture 3: Models of Solutions
Materials Science & Metallurgy Master of Philosophy, Materials Modelling, Course MP4, Thermodynamics and Phase Diagrams, H. K. D. H. Bhadeshia Lecture 3: Models of Solutions List of Symbols Symbol G M
More informationEach grain is a single crystal with a specific orientation. Imperfections
Crystal Structure / Imperfections Almost all materials crystallize when they solidify; i.e., the atoms are arranged in an ordered, repeating, 3dimensional pattern. These structures are called crystals
More informationMartensite in Steels
Materials Science & Metallurgy http://www.msm.cam.ac.uk/phasetrans/2002/martensite.html H. K. D. H. Bhadeshia Martensite in Steels The name martensite is after the German scientist Martens. It was used
More informationSilicon dioxide, SiO2
Silicon dioxide, SiO2 Sand (silica) one of the most common minerals in the earth. Main component in common glass mixed with sodium carbonate and calcium oxide (lime) to make sodalime glass for window
More informationChapter 6 An Overview of Organic Reactions
John E. McMurry www.cengage.com/chemistry/mcmurry Chapter 6 An Overview of Organic Reactions Why this chapter? To understand organic and/or biochemistry, it is necessary to know: What occurs Why and
More informationIntroduction to Materials Science, Chapter 9, Phase Diagrams. Phase Diagrams. University of Tennessee, Dept. of Materials Science and Engineering 1
Phase Diagrams University of Tennessee, Dept. of Materials Science and Engineering 1 Chapter Outline: Phase Diagrams Microstructure and Phase Transformations in Multicomponent Systems Definitions and basic
More informationChem 115 Sample Examination #1
_ Chem 115 Sample Examination #1 Student number This exam consists of seven (7) pages, including this cover page. Be sure your copy is complete before beginning your work. If this test packet is defective,
More informationBoltzmann Distribution Law
Boltzmann Distribution Law The motion of molecules is extremely chaotic Any individual molecule is colliding with others at an enormous rate Typically at a rate of a billion times per second We introduce
More informationChemistry 102 Chapter 13 CHEMICAL KINETICS
CHEMICAL KINETICS Chemical Kinetics: I. The study of the Rates of Chemical Reactions: how fast do chemical reactions proceed to form products II. The study of Reaction Mechanisms: the steps involved in
More information8. Kinetic Monte Carlo
8. Kinetic Monte Carlo [Duane Johnsons notes in web; Per Stoltze: Simulation methods in atomicscale physics; Fichthorn, Weinberg: J. Chem. Phys. 95 (1991) 1090; Bortz, Kalos, Lebowitz, J. Computational
More informationName Class Date. In the space provided, write the letter of the term or phrase that best completes each statement or best answers each question.
Assessment Chapter Test A Chapter: States of Matter In the space provided, write the letter of the term or phrase that best completes each statement or best answers each question. 1. The kineticmolecular
More informationLösungen Übung Verformung
Lösungen Übung Verformung 1. (a) What is the meaning of T G? (b) To which materials does it apply? (c) What effect does it have on the toughness and on the stress strain diagram? 2. Name the four main
More informationEnergy Transport. Focus on heat transfer. Heat Transfer Mechanisms: Conduction Radiation Convection (mass movement of fluids)
Energy Transport Focus on heat transfer Heat Transfer Mechanisms: Conduction Radiation Convection (mass movement of fluids) Conduction Conduction heat transfer occurs only when there is physical contact
More informationMajor chemistry laws. Mole and Avogadro s number. Calculating concentrations.
Major chemistry laws. Mole and Avogadro s number. Calculating concentrations. Major chemistry laws Avogadro's Law Equal volumes of gases under identical temperature and pressure conditions will contain
More informationVacuum Evaporation Recap
Sputtering Vacuum Evaporation Recap Use high temperatures at high vacuum to evaporate (eject) atoms or molecules off a material surface. Use ballistic flow to transport them to a substrate and deposit.
More informationReaction Rates and Chemical Kinetics. Factors Affecting Reaction Rate [O 2. CHAPTER 13 Page 1
CHAPTER 13 Page 1 Reaction Rates and Chemical Kinetics Several factors affect the rate at which a reaction occurs. Some reactions are instantaneous while others are extremely slow. Whether a commercial
More information[ A] 2. [ A] 2 = 2k dt. [ A] o
Chemistry 360 Dr Jean M Standard Problem Set 3 Solutions The reaction 2A " P follows secondorder kinetics The rate constant for the reaction is k350 0 4 Lmol s Determine the time required for the concentration
More informationThis is the 11th lecture of this course and the last lecture on the topic of Equilibrium Carrier Concentration.
Solid State Devices Dr. S. Karmalkar Department of Electronics and Communication Engineering Indian Institute of Technology, Madras Lecture  11 Equilibrium Carrier Concentration (Contd.) This is the 11th
More informationSOLIDIFICATION. (a)formation of stable nuclei. Growth of a stable nucleus. (c) Grain structure
SOLIDIFICATION Most metals are melted and then cast into semifinished or finished shape. Solidification of a metal can be divided into the following steps: Formation of a stable nucleus Growth of a stable
More informationCHEMISTRY STANDARDS BASED RUBRIC ATOMIC STRUCTURE AND BONDING
CHEMISTRY STANDARDS BASED RUBRIC ATOMIC STRUCTURE AND BONDING Essential Standard: STUDENTS WILL UNDERSTAND THAT THE PROPERTIES OF MATTER AND THEIR INTERACTIONS ARE A CONSEQUENCE OF THE STRUCTURE OF MATTER,
More informationComposition Solidus Liquidus (wt% Au) Temperature ( C) Temperature ( C)
10.4 Given here are the solidus and liquidus temperatures for the copper gold system. Construct the phase diagram for this system and label each region. Composition Solidus Liquidus (wt% Au) Temperature
More informationChemistry 102 Chapter 13 CHEMICAL KINETICS
CHEMICAL KINETICS Chemical Kinetics: I. The study of the Rates of Chemical Reactions: how fast do chemical reactions proceed to form products II. The study of Reaction Mechanisms: the steps involved in
More informationSemiconductor doping. Si solar Cell
Semiconductor doping Si solar Cell Two Levels of Masks  photoresist, alignment Etch and oxidation to isolate thermal oxide, deposited oxide, wet etching, dry etching, isolation schemes Doping  diffusion/ion
More informationNext, solid silicon is separated from other solid impurities by treatment with hydrogen chloride at 350 C to form gaseous trichlorosilane (SiCl 3 H):
University Chemistry Quiz 5 2014/12/25 1. (5%) What is the coordination number of each sphere in (a) a simple cubic cell, (b) a bodycentered cubic cell, and (c) a facecentered cubic cell? Assume the
More information3. Apply phase rule to the two phase field of a binary isomorphous diagram. What conclusion can be drawn?
ecture 1822: Solidification of binary alloys: Solidification of binary alloys: limits of solubility, isomorphous system, lever rule, constitutional super cooling, effect of non equilibrium cooling, eutectic,
More informationPhase Diagrams & Thermodynamics
Phase Diagrams & Thermodynamics A phase diagram is a graphical representation of the equilibrium state of a system using the intensive variables T and i while p is kept constant. The equilibrium may be
More informationProblem Set 7 Materials101 1.) You wish to develop a gold alloy (mostly gold) that can be precipitation strengthened to provide high strength  high conductivity electrical leads to integrated circuits
More informationOxide Growth. 1. Introduction
Oxide Growth. Introduction Development of highquality silicon dioxide (SiO 2 ) has helped to establish the dominance of silicon in the production of commercial integrated circuits. Among all the various
More informationAerogel an excellent thermal insulator (known as frozen smoke)
Aerogel an excellent thermal insulator (known as frozen smoke) 2 Thermal images of a dog (top) and a snake wrapped around a human arm (bottom) Thermal Properties (1) Heat Capacity Heat Capacity When heated,
More informationLecture 3: Electron statistics in a solid
Lecture 3: Electron statistics in a solid Contents Density of states. DOS in a 3D uniform solid.................... 3.2 DOS for a 2D solid........................ 4.3 DOS for a D solid........................
More informationTheory of Chromatography
Theory of Chromatography The Chromatogram A chromatogram is a graph showing the detector response as a function of elution time. The retention time, t R, for each component is the time needed after injection
More informationConcepts of Stress and Strain
CHAPTER 6 MECHANICAL PROPERTIES OF METALS PROBLEM SOLUTIONS Concepts of Stress and Strain 6.4 A cylindrical specimen of a titanium alloy having an elastic modulus of 107 GPa (15.5 10 6 psi) and an original
More informationChapter 13 Rates of Reaction
Chapter 13 Rates of Reaction Chemical Kinetics: Rates of Chemical Reactions & Factors that Affect Rates of Reactions How fast does a chemical reaction occur? rates of reactants consumed rates of products
More informationSemiconductors, diodes, transistors
Semiconductors, diodes, transistors (Horst Wahl, QuarkNet presentation, June 2001) Electrical conductivity! Energy bands in solids! Band structure and conductivity Semiconductors! Intrinsic semiconductors!
More informationLecture 14. Chapter 81
Lecture 14 Fatigue & Creep in Engineering Materials (Chapter 8) Chapter 81 Fatigue Fatigue = failure under applied cyclic stress. specimen compression on top bearing bearing motor counter flex coupling
More information5.6 Isobaric thermal expansion and isothermal compression (Hiroshi Matsuoka)
5.6 Isobaric thermal expansion and isothermal compression Hiroshi Matsuoka 1 5.6.2 he coefficient of thermal expansion as a response function to a temperature change he coefficient of thermal expansion
More informationLecture 19: Eutectoid Transformation in Steels: a typical case of Cellular
Lecture 19: Eutectoid Transformation in Steels: a typical case of Cellular Precipitation Today s topics Understanding of Cellular transformation (or precipitation): when applied to phase transformation
More information1A Rate of reaction. AS Chemistry introduced the qualitative aspects of rates of reaction. These include:
1A Rate of reaction AS Chemistry introduced the qualitative aspects of rates of reaction. These include: Collision theory Effect of temperature Effect of concentration Effect of pressure Activation energy
More informationCandidate Style Answer
Candidate Style Answer Chemistry A Unit F321 Atoms, Bonds and Groups High banded response This Support Material booklet is designed to accompany the OCR GCE Chemistry A Specimen Paper F321 for teaching
More informationThe MaxwellBoltzmann Distribution
The MaxwellBoltzmann Distribution Gases are composed of atoms or molecules. These atoms or molecules do not really interact with each other except through collisions. In many cases, we may think of a
More information